#------------------------------------------------------------------------------
#$Date: 2016-03-26 19:42:49 +0100 (Sat 26 de Mar de 2016) $
#$Revision: 180445 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/14/7211445.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7211445
loop_
_publ_author_name
'Yang, Bing-Ping'
'Xu, Xiang'
'Huang, Chao'
'Mao, Jiang-Gao'
_publ_section_title
;
 K4TM4(V2O7)2(IO3)4(H2O) (TM = Zn, Ni, Co): a series of quinary mixed
 metal--vanadium(v)--iodates
;
_journal_issue                   48
_journal_name_full               CrystEngComm
_journal_page_first              10464
_journal_paper_doi               10.1039/c3ce41653d
_journal_volume                  15
_journal_year                    2013
_chemical_formula_moiety         '2(I2 Ni2 O13 V2), 2(O0.50), 4(K)'
_chemical_formula_sum            'H2 I4 K4 Ni4 O27 V4'
_chemical_formula_weight         1536.62
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   5.5379(2)
_cell_length_b                   5.5379(2)
_cell_length_c                   25.931(2)
_cell_measurement_reflns_used    1876
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.48
_cell_measurement_theta_min      4.25
_cell_volume                     688.72(6)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2007)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2007)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2007)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0656
_diffrn_reflns_av_sigmaI/netI    0.0331
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       32
_diffrn_reflns_limit_l_min       -33
_diffrn_reflns_number            5852
_diffrn_reflns_theta_full        27.48
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_min         4.25
_exptl_absorpt_coefficient_mu    9.159
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.4622
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   Higashi
_exptl_crystal_colour            'light green'
_exptl_crystal_density_diffrn    3.705
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'hexagonal plate'
_exptl_crystal_F_000             710
_exptl_crystal_size_max          0.11
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.03
_refine_diff_density_max         0.859
_refine_diff_density_min         -1.406
_refine_diff_density_rms         0.184
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.391
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     38
_refine_ls_number_reflns         542
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.391
_refine_ls_R_factor_all          0.0521
_refine_ls_R_factor_gt           0.0512
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0152P)²+8.1237P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0968
_refine_ls_wR_factor_ref         0.0972
_reflns_number_gt                538
_reflns_number_total             542
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3ce41653d.cif
_cod_data_source_block           K4Ni4(V2O7)2(IO3)4(H2O)
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_sg_symbol_H-M      P6(3)/m
_cod_database_code               7211445
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x-y, x, z+1/2'
'-y, x-y, z'
'-x, -y, z+1/2'
'-x+y, -x, z'
'y, -x+y, z+1/2'
'-x, -y, -z'
'-x+y, -x, -z-1/2'
'y, -x+y, -z'
'x, y, -z-1/2'
'x-y, x, -z'
'-y, x-y, -z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
K1 K 0.3333 0.6667 0.2500 0.035(3) Uani 0.68(2) 6 d SP
K2 K 0.3333 0.6667 -0.0188(2) 0.055(2) Uani 0.658(10) 3 d SP
Ni1 Ni 0.3333 0.6667 0.11578(7) 0.0170(4) Uani 1 3 d S
V1 V 0.6667 0.3333 0.18147(8) 0.0121(5) Uani 1 3 d S
I1 I 0.0000 1.0000 0.10291(3) 0.0148(3) Uani 1 3 d S
O1 O 0.2157(11) 0.8911(11) 0.0689(2) 0.0197(12) Uani 1 1 d .
O2 O 0.6667 0.3333 0.2500 0.054(6) Uani 1 6 d S
O3 O 0.4364(13) 0.4235(12) 0.1596(2) 0.0224(12) Uani 1 1 d .
O1W O 0.0000 1.0000 0.2500 0.025(6) Uani 0.50 6 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
I I -0.4742 1.8119 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 K1 O3 145.78(9) 5_565 12_666
O3 K1 O3 61.26(18) 5_565 3_665
O3 K1 O3 107.9(2) 12_666 3_665
O3 K1 O3 107.9(2) 5_565 8_566
O3 K1 O3 61.26(18) 12_666 8_566
O3 K1 O3 145.78(9) 3_665 8_566
O3 K1 O3 61.26(18) 5_565 .
O3 K1 O3 145.78(9) 12_666 .
O3 K1 O3 61.26(18) 3_665 .
O3 K1 O3 145.78(9) 8_566 .
O3 K1 O3 145.78(9) 5_565 10_556
O3 K1 O3 61.26(18) 12_666 10_556
O3 K1 O3 145.78(9) 3_665 10_556
O3 K1 O3 61.26(18) 8_566 10_556
O3 K1 O3 107.9(2) . 10_556
O3 K1 O2 99.82(12) 5_565 1_565
O3 K1 O2 55.05(11) 12_666 1_565
O3 K1 O2 55.05(11) 3_665 1_565
O3 K1 O2 99.82(12) 8_566 1_565
O3 K1 O2 113.73(12) . 1_565
O3 K1 O2 113.73(12) 10_556 1_565
O3 K1 O2 55.05(11) 5_565 1_455
O3 K1 O2 113.73(12) 12_666 1_455
O3 K1 O2 113.73(12) 3_665 1_455
O3 K1 O2 55.05(11) 8_566 1_455
O3 K1 O2 99.82(12) . 1_455
O3 K1 O2 99.82(12) 10_556 1_455
O2 K1 O2 120.0 1_565 1_455
O3 K1 O1W 66.27(12) 5_565 .
O3 K1 O1W 80.18(12) 12_666 .
O3 K1 O1W 80.18(12) 3_665 .
O3 K1 O1W 66.27(12) 8_566 .
O3 K1 O1W 124.95(11) . .
O3 K1 O1W 124.95(11) 10_556 .
O2 K1 O1W 60.0 1_565 .
O2 K1 O1W 60.0 1_455 .
O3 K1 O1W 124.95(11) 5_565 1_655
O3 K1 O1W 66.27(12) 12_666 1_655
O3 K1 O1W 66.27(12) 3_665 1_655
O3 K1 O1W 124.95(11) 8_566 1_655
O3 K1 O1W 80.18(12) . 1_655
O3 K1 O1W 80.18(12) 10_556 1_655
O2 K1 O1W 60.0 1_565 1_655
O2 K1 O1W 180.0 1_455 1_655
O1W K1 O1W 120.0 . 1_655
O3 K1 O1W 80.18(12) 5_565 1_545
O3 K1 O1W 124.95(11) 12_666 1_545
O3 K1 O1W 124.95(11) 3_665 1_545
O3 K1 O1W 80.18(12) 8_566 1_545
O3 K1 O1W 66.27(12) . 1_545
O3 K1 O1W 66.27(12) 10_556 1_545
O2 K1 O1W 180.0 1_565 1_545
O2 K1 O1W 60.0 1_455 1_545
O1W K1 O1W 120.0 . 1_545
O1W K1 O1W 120.0 1_655 1_545
O3 K1 O2 113.73(12) 5_565 .
O3 K1 O2 99.82(12) 12_666 .
O3 K1 O2 99.82(12) 3_665 .
O3 K1 O2 113.73(12) 8_566 .
O3 K1 O2 55.05(11) . .
O3 K1 O2 55.05(11) 10_556 .
O2 K1 O2 120.0 1_565 .
O2 K1 O2 120.0 1_455 .
O1W K1 O2 180.0 . .
O1W K1 O2 60.0 1_655 .
O1W K1 O2 60.0 1_545 .
O1 K2 O1 100.1(2) 9_455 7_675
O1 K2 O1 100.1(2) 9_455 11_655
O1 K2 O1 100.1(2) 7_675 11_655
O1 K2 O1 88.3(2) 9_455 .
O1 K2 O1 106.94(14) 7_675 .
O1 K2 O1 149.8(2) 11_655 .
O1 K2 O1 149.8(2) 9_455 5_565
O1 K2 O1 88.3(2) 7_675 5_565
O1 K2 O1 106.94(14) 11_655 5_565
O1 K2 O1 61.6(2) . 5_565
O1 K2 O1 106.94(14) 9_455 3_665
O1 K2 O1 149.8(2) 7_675 3_665
O1 K2 O1 88.3(2) 11_655 3_665
O1 K2 O1 61.6(2) . 3_665
O1 K2 O1 61.6(2) 5_565 3_665
O1 K2 O1 55.4(2) 9_455 7_565
O1 K2 O1 129.2(3) 7_675 7_565
O1 K2 O1 52.4(2) 11_655 7_565
O1 K2 O1 114.77(13) . 7_565
O1 K2 O1 136.53(17) 5_565 7_565
O1 K2 O1 78.50(19) 3_665 7_565
O1 K2 O1 52.4(2) 9_455 11_665
O1 K2 O1 55.4(2) 7_675 11_665
O1 K2 O1 129.2(3) 11_655 11_665
O1 K2 O1 78.50(19) . 11_665
O1 K2 O1 114.77(13) 5_565 11_665
O1 K2 O1 136.53(17) 3_665 11_665
O1 K2 O1 105.73(15) 7_565 11_665
O1 K2 O1 129.2(3) 9_455 9
O1 K2 O1 52.4(2) 7_675 9
O1 K2 O1 55.4(2) 11_655 9
O1 K2 O1 136.53(17) . 9
O1 K2 O1 78.50(19) 5_565 9
O1 K2 O1 114.77(13) 3_665 9
O1 K2 O1 105.73(15) 7_565 9
O1 K2 O1 105.73(15) 11_665 9
O1 K2 K2 96.97(13) 9_455 7_675
O1 K2 K2 53.82(14) 7_675 7_675
O1 K2 K2 151.15(17) 11_655 7_675
O1 K2 K2 53.12(18) . 7_675
O1 K2 K2 64.77(19) 5_565 7_675
O1 K2 K2 108.8(3) 3_665 7_675
O1 K2 K2 151.93(12) 7_565 7_675
O1 K2 K2 50.00(13) 11_665 7_675
O1 K2 K2 95.85(11) 9 7_675
O1 K2 K2 53.82(14) 9_455 7_565
O1 K2 K2 151.15(17) 7_675 7_565
O1 K2 K2 96.97(13) 11_655 7_565
O1 K2 K2 64.77(19) . 7_565
O1 K2 K2 108.8(3) 5_565 7_565
O1 K2 K2 53.12(18) 3_665 7_565
O1 K2 K2 50.00(13) 7_565 7_565
O1 K2 K2 95.85(11) 11_665 7_565
O1 K2 K2 151.93(12) 9 7_565
K2 K2 K2 111.88(19) 7_675 7_565
O1 K2 K2 151.15(17) 9_455 7_665
O1 K2 K2 96.97(13) 7_675 7_665
O1 K2 K2 53.82(14) 11_655 7_665
O1 K2 K2 108.8(3) . 7_665
O1 K2 K2 53.12(18) 5_565 7_665
O1 K2 K2 64.77(19) 3_665 7_665
O1 K2 K2 95.85(11) 7_565 7_665
O1 K2 K2 151.93(12) 11_665 7_665
O1 K2 K2 50.00(13) 9 7_665
K2 K2 K2 111.88(19) 7_675 7_665
K2 K2 K2 111.88(19) 7_565 7_665
O3 Ni1 O3 92.2(2) 3_665 5_565
O3 Ni1 O3 92.2(2) 3_665 .
O3 Ni1 O3 92.2(2) 5_565 .
O3 Ni1 O1 176.6(2) 3_665 3_665
O3 Ni1 O1 91.2(2) 5_565 3_665
O3 Ni1 O1 87.8(2) . 3_665
O3 Ni1 O1 91.2(2) 3_665 .
O3 Ni1 O1 87.8(2) 5_565 .
O3 Ni1 O1 176.6(2) . .
O1 Ni1 O1 88.8(2) 3_665 .
O3 Ni1 O1 87.8(2) 3_665 5_565
O3 Ni1 O1 176.6(2) 5_565 5_565
O3 Ni1 O1 91.2(2) . 5_565
O1 Ni1 O1 88.8(2) 3_665 5_565
O1 Ni1 O1 88.8(2) . 5_565
O3 Ni1 K1 56.31(16) 3_665 .
O3 Ni1 K1 56.31(16) 5_565 .
O3 Ni1 K1 56.31(16) . .
O1 Ni1 K1 126.08(15) 3_665 .
O1 Ni1 K1 126.08(15) . .
O1 Ni1 K1 126.08(15) 5_565 .
O3 Ni1 K2 123.69(16) 3_665 .
O3 Ni1 K2 123.69(16) 5_565 .
O3 Ni1 K2 123.69(16) . .
O1 Ni1 K2 53.92(15) 3_665 .
O1 Ni1 K2 53.92(15) . .
O1 Ni1 K2 53.92(15) 5_565 .
K1 Ni1 K2 180.0 . .
O3 V1 O3 109.3(2) 3_655 5_665
O3 V1 O3 109.3(2) 3_655 .
O3 V1 O3 109.3(2) 5_665 .
O3 V1 O2 109.7(2) 3_655 .
O3 V1 O2 109.7(2) 5_665 .
O3 V1 O2 109.7(2) . .
O3 V1 K1 112.8(2) 3_655 1_655
O3 V1 K1 50.62(19) 5_665 1_655
O3 V1 K1 137.5(2) . 1_655
O2 V1 K1 60.94(3) . 1_655
O3 V1 K1 50.62(19) 3_655 1_545
O3 V1 K1 137.5(2) 5_665 1_545
O3 V1 K1 112.8(2) . 1_545
O2 V1 K1 60.94(3) . 1_545
K1 V1 K1 98.40(3) 1_655 1_545
O3 V1 K1 137.5(2) 3_655 .
O3 V1 K1 112.8(2) 5_665 .
O3 V1 K1 50.62(19) . .
O2 V1 K1 60.94(3) . .
K1 V1 K1 98.40(3) 1_655 .
K1 V1 K1 98.40(3) 1_545 .
O1 I1 O1 98.4(2) 5_465 3_675
O1 I1 O1 98.4(2) 5_465 .
O1 I1 O1 98.4(2) 3_675 .
O1 I1 K2 41.83(17) 5_465 7_565
O1 I1 K2 115.82(19) 3_675 7_565
O1 I1 K2 59.22(18) . 7_565
O1 I1 K2 59.22(17) 5_465 7_575
O1 I1 K2 41.83(17) 3_675 7_575
O1 I1 K2 115.82(19) . 7_575
K2 I1 K2 91.35(11) 7_565 7_575
O1 I1 K2 115.82(19) 5_465 7_675
O1 I1 K2 59.22(18) 3_675 7_675
O1 I1 K2 41.83(17) . 7_675
K2 I1 K2 91.35(11) 7_565 7_675
K2 I1 K2 91.35(11) 7_575 7_675
I1 O1 Ni1 111.9(3) . .
I1 O1 K2 112.5(2) . 7_675
Ni1 O1 K2 112.9(2) . 7_675
I1 O1 K2 151.0(3) . .
Ni1 O1 K2 89.8(2) . .
K2 O1 K2 73.06(14) 7_675 .
I1 O1 K2 92.9(2) . 7_565
Ni1 O1 K2 95.05(19) . 7_565
K2 O1 K2 129.2(3) 7_675 7_565
K2 O1 K2 65.23(13) . 7_565
V1 O2 V1 180.0 . 8_666
V1 O2 K1 90.0 . 1_655
V1 O2 K1 90.0 8_666 1_655
V1 O2 K1 90.0 . 1_545
V1 O2 K1 90.0 8_666 1_545
K1 O2 K1 120.0 1_655 1_545
V1 O2 K1 90.0 . .
V1 O2 K1 90.0 8_666 .
K1 O2 K1 120.0 1_655 .
K1 O2 K1 120.0 1_545 .
V1 O3 Ni1 152.0(4) . .
V1 O3 K1 102.7(2) . .
Ni1 O3 K1 87.7(2) . .
K1 O1W K1 120.0 . 1_565
K1 O1W K1 120.0 . 1_455
K1 O1W K1 120.0 1_565 1_455
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
K1 O3 2.898(6) 5_565
K1 O3 2.898(6) 12_666
K1 O3 2.898(6) 3_665
K1 O3 2.898(6) 8_566
K1 O3 2.898(6) .
K1 O3 2.898(6) 10_556
K1 O2 3.19731(11) 1_565
K1 O2 3.19731(11) 1_455
K1 O1W 3.19731(11) .
K1 O1W 3.19731(11) 1_655
K1 O1W 3.19731(11) 1_545
K1 O2 3.19731(11) .
K2 O1 2.795(6) 9_455
K2 O1 2.795(6) 7_675
K2 O1 2.795(6) 11_655
K2 O1 2.820(7) .
K2 O1 2.820(7) 5_565
K2 O1 2.820(7) 3_665
K2 O1 3.330(6) 7_565
K2 O1 3.330(6) 11_665
K2 O1 3.330(6) 9
K2 K2 3.342(4) 7_675
K2 K2 3.342(4) 7_565
K2 K2 3.342(4) 7_665
Ni1 O3 2.049(6) 3_665
Ni1 O3 2.049(6) 5_565
Ni1 O3 2.049(6) .
Ni1 O1 2.062(5) 3_665
Ni1 O1 2.062(5) .
Ni1 O1 2.062(5) 5_565
V1 O3 1.683(6) 3_655
V1 O3 1.683(6) 5_665
V1 O3 1.683(6) .
V1 O2 1.777(2) .
V1 K1 3.6579(10) 1_655
V1 K1 3.6579(10) 1_545
I1 O1 1.813(5) 5_465
I1 O1 1.813(5) 3_675
I1 O1 1.813(5) .
I1 K2 3.871(4) 7_565
I1 K2 3.871(4) 7_575
I1 K2 3.871(4) 7_675
O1 K2 2.795(6) 7_675
O1 K2 3.330(6) 7_565
O2 V1 1.777(2) 8_666
O2 K1 3.19731(11) 1_655
O2 K1 3.19731(11) 1_545
O1W K1 3.19731(11) 1_565
O1W K1 3.19731(11) 1_455
